DOI: 10.17188/1722505
title: Materials Data on Li32Ti13Cr3O48 by Materials Project

description: Li32Ti13Cr3O48 is beta Polonium-derived structured and crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are thirty-two inequivalent Li sites. In the first Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three TiO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.09–2.28 Å. In the second Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with two equivalent CrO6 octahedra, edges with four TiO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Li–O bond distances ranging from 2.10–2.14 Å. In the third Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.05–2.21 Å. In the fourth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–9°. There are a spread of Li–O bond distances ranging from 2.10–2.22 Å. In the fifth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, edges with two TiO6 octahedra, edges with two CrO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.11–2.21 Å. In the sixth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two TiO6 octahedra, corners with two CrO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.09–2.24 Å. In the seventh Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with five TiO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are a spread of Li–O bond distances ranging from 2.12–2.16 Å. In the eighth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two TiO6 octahedra, corners with two CrO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–8°. There are a spread of Li–O bond distances ranging from 2.04–2.24 Å. In the ninth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two TiO6 octahedra, corners with two CrO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Li–O bond distances ranging from 2.08–2.27 Å. In the tenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six TiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are a spread of Li–O bond distances ranging from 2.11–2.14 Å. In the eleventh Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Li–O bond distances ranging from 2.09–2.22 Å. In the twelfth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Li–O bond distances ranging from 2.09–2.23 Å. In the thirteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with two equivalent CrO6 octahedra, edges with four TiO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Li–O bond distances ranging from 2.10–2.14 Å. In the fourteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–8°. There are a spread of Li–O bond distances ranging from 2.05–2.21 Å. In the fifteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.11–2.22 Å. In the sixteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two TiO6 octahedra, corners with two CrO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.09–2.23 Å. In the seventeenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with five TiO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are a spread of Li–O bond distances ranging from 2.12–2.15 Å. In the eighteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two TiO6 octahedra, corners with two CrO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–8°. There are a spread of Li–O bond distances ranging from 2.04–2.25 Å. In the nineteenth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three TiO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–8°. There are a spread of Li–O bond distances ranging from 2.05–2.20 Å. In the twentieth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with two TiO6 octahedra, corners with two CrO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.08–2.27 Å. In the twenty-first Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three TiO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–9°. There are a spread of Li–O bond distances ranging from 2.08–2.26 Å. In the twenty-second Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with two equivalent CrO6 octahedra, edges with four TiO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Li–O bond distances ranging from 2.09–2.14 Å. In the twenty-third Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Li–O bond distances ranging from 2.10–2.23 Å. In the twenty-fourth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.05–2.22 Å. In the twenty-fifth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six TiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are a spread of Li–O bond distances ranging from 2.11–2.14 Å. In the twenty-sixth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, edges with two TiO6 octahedra, edges with two CrO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.10–2.22 Å. In the twenty-seventh Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three TiO6 octahedra, edges with four TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Li–O bond distances ranging from 2.10–2.22 Å. In the twenty-eighth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.09–2.24 Å. In the twenty-ninth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with five TiO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are a spread of Li–O bond distances ranging from 2.12–2.16 Å. In the thirtieth Li site, Li is bonded to six O atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 6–8°. There are a spread of Li–O bond distances ranging from 2.05–2.24 Å. In the thirty-first Li site, Li is bonded to six O atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four TiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three TiO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Li–O bond distances ranging from 2.10–2.24 Å.